- Home
- Documents
- A Stochastic Reliability Model for Application in a ... ?· A Stochastic Reliability Model for Application…

Published on

28-Jul-2018View

212Download

0

Embed Size (px)

Transcript

<ul><li><p>2316 </p><p>Abstract Currently, there are a lot of research activities dealing with gam-ma titanium aluminide (-TiAl) alloys as new materials for low pressure turbine (LPT) blades. Even though the scatter in me-chanical properties of such intermetallic alloys is more distinctive as in conventional metallic alloys, stochastic investigations on -TiAl alloys are very rare. For this reason, we analyzed the scatter in static and dynamic mechanical properties of the cast alloy Ti-48Al-2Cr-2Nb. It was found that this alloy shows a size effect in strength which is less pronounced than the size effect of brittle materials. A weakest-link approach is enhanced for describing a scalable size effect under multiaxial stress states and implemented in a post processing tool for reliability analysis of real components. The presented approach is a first applicable reliability model for semi-brittle materials. The developed reliability tool was integrat-ed into a multidisciplinary optimization of the geometry of a LPT blade. Some processes of the optimization were distributed in a wide area network, so that specialized tools for each discipline could be employed. The optimization results show that it is possi-ble to increase the aerodynamic efficiency and the structural me-chanics reliability at the same time, while ensuring the blade can be manufactured in an investment casting process. Keywords Size effect, weakest link, investment casting. </p><p> A Stochastic Reliability Model for Application in a Multidisciplinary Optimization of a Low Pressure Turbine Blade Made of Titanium Aluminide </p><p>Christian Dresbach a Thomas Becker b Stefan Reh c Janine Wischek d Sascha Zur e Clemens Buske f Thomas Schmidt g Ruediger Tiefers h a DLR, Linder Hoehe, 51147 Cologne, Germany, Christian.Dresbach@dlr.de b DLR, Linder Hoehe, 51147 Cologne, Germany, T.Becker@dlr.de c DLR, Linder Hoehe, 51147 Cologne, Germany, Stefan.Reh@dlr.de d DLR, Linder Hoehe, 51147 Cologne, Germany, Janine.Wischek@dlr.de e DLR, Linder Hoehe, 51147 Cologne, Germany, Sascha.Zur@dlr.de f DLR, Bunsenstr. 10, 37073 Goettingen, Germany, Clemens.Buske@dlr.de g DLR, Pfaffenwaldring 38-40, 70569 Stuttgart, Germany, Thomas.Schmidt@dlr.de h Access e.V., Juelicherstr. 322, 52070 Aachen, Germany, R.Tiefers@access-technology.de http://dx.doi.org/10.1590/1679-78252521 Received 09.10.2015 In revised form 02.05.2016 Accepted 10.06.2016 Available online 27.06.2016 </p></li><li><p>C. Dresbach et al. / A Stochastic Reliability Model for Application in a Multidisciplinary Optimization of a Low Pressure Turbine Blade 2317 </p><p>Latin American Journal of Solids and Structures 13 (2016) 2316-2332 </p><p>1 INTRODUCTION </p><p>The introduction of gamma titanium aluminide (-TiAl) alloys, as a material for low pressure tur-bine (LPT) blades, is one of the most promising attempts for saving weight and consequently fuel of aero engines like shown in Appel (2011). For this reason, there are a lot of activities in industrial and scientific research dealing with different -TiAl alloys and since some years first blades made of -TiAl alloys are used in real airplanes, see also the press releases of MTU (2015), Snecma (2015) and GE (2015). </p><p>Due to the high specific modulus and strength, the weight of a LPT blade made of a -TiAl al-loy would be approximately half of a conventional blade made of a nickel based alloy. This weight reduction also leads to much smaller centrifugal forces acting on the blades and consequently on the disc, which holds the blades. An additional re-design to decrease the weight of disc and other fixa-tion components should be possible. Thus, not only the lightweight -TiAl blades, but also the ef-fects on other engine parts could reduce the total engine weight and accordingly save a significant amount of fuel. </p><p>Most of current investigations are related to material characterization in a temperature range of 500C - 900C (Recina and Karlsson, 2000 / Henaff and Gloanec, 2005 / Appel et al., 2010), micro-mechanical modeling (Chakraborty and Earthman, 1998 / Kabir et al., 2010), or classical compo-nent design processes based on deterministic approaches. However, probabilistic aspects should be considered when developing -TiAl turbine blades due to the quasi-brittle behavior of these alloys at room temperature. Classical stochastic approaches like Monte Carlo are inefficient and cannot be used to directly address failure probabilities of technical components smaller than 10-4, when the component loading needs to be calculated by time-consuming numerical methods like the finite ele-ment method. There are well-known probabilistic methods, see for example Munz and Fett (1999) or Nemeth et al. (2005), for calculating the failure probability of brittle components based on the weakest link theory developed by Weibull (1951). Still, these methods cannot be directly applied for quasi-brittle materials like -TiAl. Therefore, in this work we present a modified weakest link ap-proach representing the experimental findings of a commercially available cast -TiAl alloy and show its applicability for calculating the component failure probability. </p><p>When substituting a low pressure turbine blade made of a nickel alloy with one made of a -TiAl alloy, the original geometry of the blade needs to be modified due to the different material properties and specific manufacturing restrictions. For this purpose, it is necessary to consider the aerodynamic efficiency and the structural mechanics reliability as well as manufacturing limitations and expenses. Usually, aspects of aerodynamic performance and deterministic structural mechanics are treated by the original equipment manufacturer (OEM), while the manufacturability is in the hand of the component supplier and stochastic aspects are neglected so far. Since manufacturing aspects are assessed only at the end of such a design process, complete aerodynamic re-designs are often necessary, resulting in a time-consuming iterative design process. Thus, a blade design gener-ated in this sequential way would probably not lead to an optimal geometry. Accordingly, we pre-sent a fully automated and multidisciplinary simulation process chain. This process chain is used in a geometry optimization of a low pressure turbine blade to demonstrate the feasibility to increase its aerodynamic efficiency and the structural mechanics reliability. At the same time it is ensured that the resulting geometry can be manufactured by an investment casting process as well. </p></li><li><p>2318 C. Dresbach et al. / A Stochastic Reliability Model for Application in a Multidisciplinary Optimization of a Low Pressure Turbine Blade </p><p>Latin American Journal of Solids and Structures 13 (2016) 2316-2332 </p><p>2 STATIC AND FATIGUE STRENGTH OF CAST TI-48AL-2CR-2NB </p><p>In this investigation we characterized the static and fatigue material behavior of the gamma titani-um aluminide alloy Ti-48Al-2Cr-2Nb, which is already used for turbine blades in aircraft engines. The specimens were prepared by creating round bars with an investment casting process resulting in a duplex microstructure. After applying a hot isostatic pressing (HIP) process, the bars were lathed to the final geometry. The specimens used for the fatigue experiments were additionally pol-ished before testing. </p><p>Three different specimen geometries were developed. All specimens are round tensile bars with a parallel section in the middle. The enlargement sections of the specimens were defined by a b-spline formulation instead of a classical radius to minimize the stress concentration without enlarging the specimens too much. The optimal spline definition was identified by finite element simulations for each specimen size. The parameters of the developed geometries are listed in Table 1. Tensile tests were performed using a 100 kN Instron spindle testing machine with a load cell scaled to 30 kN, while the strain was measured by a Fiedler laser extensometer. Different tensile test procedures were used for characterizing the elastic and the elasto-plastic material behavior. The Youngs modu-lus is determined from an un- and reloading segment after reaching a nominal stress slightly over the initial yield stress. 20 samples with a diameter of D = 4 mm were used for this investigation. For characterizing the elasto-plastic behavior the nominal stresses and strains were determined while loading until fracture in a displacement controlled experiment. For each of the three geome-tries, 20 samples were used in this test series. </p><p>Geometry parameters Diameter in </p><p>parallel section (mm) </p><p>Length of parallel section </p><p>(mm) </p><p>Volume of parallel section </p><p>(mm3) </p><p>Type of fixation thread </p><p>Length between </p><p>threads (mm) </p><p>Spline parameter </p><p>2 8 31 M8x1 29 mm 0.68 4 10 125 M12x1 39 mm 0.75 6 15 424 M16x1 49 mm 0.64 </p><p>Sketch and photo </p><p>Table 1: Geometry parameters of the specimens for tensile tests and fatigue experiments; sketch with colored stress levels and photograph of a specimen with a diameter in parallel section of D = 4mm. </p><p> The experimentally determined Youngs modulus is normal distributed with a mean value of </p><p>174 GPa and a standard deviation of 14 GPa. After an initial yield stress of 357 16 MPa (mean value standard deviation) some amount of hardening occurs until the strength of 437 13 MPa is reached. The maximum plastic strain is determined to be 0.94 0.18 %. The fracture positions </p></li><li><p>C. Dresbach et al. / A Stochastic Reliability Model for Application in a Multidisciplinary Optimization of a Low Pressure Turbine Blade 2319 </p><p>Latin American Journal of Solids and Structures 13 (2016) 2316-2332 </p><p>are uniformly distributed and not localized in the transition section between the parallel section and the fixation of the specimen. From this, it is concluded that the geometry optimization was success-ful. The probability plot of the tensile strength values in Figure 1 (left) shows a size effect indicat-ing that the larger the loaded volume the smaller the measured strength value. Additionally, it is shown that the size effect is less pronounced than the classical size effect of brittle materials, which is implicitly included in Weibulls weakest link theory, as shown in Munz and Fett (1999). Here, the failure probability Pf is expressed by the applied stress , the materials characteristic strength 0, the Weibull modulus m, the loaded volume V and the reference volume V0 as shown in the follow-ing equation: </p><p>m</p><p>f0 0</p><p>VP 1 exp</p><p>V</p><p> s = - - s (1) </p><p>In Figure 1 (left) the expected strength distribution for the samples with D = 2 mm and D = 6 mm are calculated from the results of the samples with D = 4 mm assuming a classical size effect with the loaded volume being equal to the nominal volume of the sample. The fact that Ti-48Al-2Cr-2Nb shows a reduced size effect is not surprising, since this intermetallic compound behaves nearly brittle with a small amount of plastic deformation. A similar effect of a less pro-nounced size effect has already been shown by Padgett et al. (1995) for carbon fibers and by Curtin (1999) for fiber reinforced composites. Both groups introduced a scaling parameter on the size ratio, which is a length ratio for these fiber materials. Transferred to the case of volume related failure, as we expect for an intermetallic alloy, equation (1) is extended by a scaling parameter , which has a range from zero to one: </p><p>m</p><p>f0 0</p><p>VP 1 exp with 0 1</p><p>V</p><p>a s = - - a s </p><p> (2)</p><p>Using this approach, it is possible to rebuild the experimental findings of a moderate size effect in strength, see Figure 1 (right). The determined parameters for this case are 0 = 443 MPa, m = 44, V0 = 125 mm3, = 0.56. All values are listed in Table 2. </p><p>Identified model parameters </p><p> V0 (mm3) 0 </p><p>(MPa) m </p><p>tensile test (nominal) 125 443 44 0.56 fatigue test (nominal), R = 0.1, N = 6.0e+6 125 407 (44) (0.56) </p><p>tensile test (125) 453 31 0.30 fatigue test, R = 0.1, N = 6.0e+6 (125) 413 (31) (0.30) </p><p>strength, cast flat sample (125) 382 28 0.74 fatigue, cast flat sample, R = 0.1, N = 1.0e+6 (125) 332 (28) (0.74) </p><p>Table 2: Identified model parameters from different experiments for a defined reference volume V0. Values in round brackets () are taken from the experiments listed the lines above. </p></li><li><p>2320 C. Dresbach et al. / A Stochastic Reliability Model for Application in a Multidisciplinary Optimization of a Low Pressure Turbine Blade </p><p>Latin American Journal of Solids and Structures 13 (2016) 2316-2332 </p><p>Figure 1: Probability plot of the measured strength values for three different specimen sizes (D: 2 mm, 4 mm, 6 mm) in comparison with the classical size effect of brittle materials calculated from the mean sample size (left) </p><p>and in comparison with the modified size effect following the Curtin model (right). </p><p> Additional load controlled fatigue tests with a stress ratio of R = min / max = 0.1 were per-</p><p>formed using specimens with a diameter of D = 4 mm in a servo hydraulic testing machine at fre-quencies of 10 Hz and 30 Hz. In Figure 2 (left) the cycles to failure are plotted against the maxi-mum applied stress for the fatigue experiments. The tensile strength data as well as the initial yield stress data are additionally represented for comparison. The fatigue data shows that the fatigue regime for this cast -TiAl alloy is very narrow and directly below the tensile strength regime. This leads to a great scatter in the fatigue behavior. When creating a probability plot of the fatigue strength data for a defined number of cycles to failure, it is possible to adopt the former described probabilistic strength model to rebuild this fatigue behavior. In Figure 2 (right) the estimated fa-tigue probability data for 6 million cycles to failure is in a good agreement with the scaled probabil-istic strength model with 0 = 407 MPa, when the other parameters are not changed. </p><p>Figure 2: Comparison of the fatigue data, the tensile strength data and the initial yield stress data (left); estimated probability plot of fatigue strength for 6 million cycles with R = 0.1 in comparison to the tensile strength. </p></li><li><p>C. Dresbach et al. / A Stochastic Reliability Model for Application in a Multidisciplinary Optimization of a Low Pressure Turbine Blade 2321 </p><p>Latin American Journal of Solids and Structures 13 (2016) 2316-2332 </p><p>3 A MODIFIED FAILURE CRITERION AND ITS IMPLEMENTATION IN A RELIABILITY TOOL </p><p>The former described model is able to rebuild the experimental findings of an assumed uniaxial experiment with a constant stress level in the tested volume. For applying it in a reliability assess-ment of a real technical component, it is necessary to enhance the model to deal with multiaxial stress states and non-uniform stresses. Furthermore, the model needs to be independent of the dis-cretization, when the stress level is in a converged state. For this purpose, a post processing tool called HYPRA was developed. This reliability tool acts in principle like other tools such as CaresLife from NASA (Nemeth et al., 2005) or...</p></li></ul>